International Journal of Engineering Research and Developmente-ISSN: 2278-067X, p-ISSN: 2278-800X, www.ijerd.comVolume 7, Issue 1 (May 2013), PP. 06-136Effect of W/C Ratio on Workability and MechanicalProperties of High Strength Self Compacting Concrete(M70 Grade)Mallikarjuna Reddy V1, Seshagiri Rao M V2, Srilakshmi P2, Sateesh Kumar B21Department of Civil Engineering, Gokaraju Rangaraju Institute of Engineering and Technology,Hyderabad, India2Department of Civil Engineering, JNTUH College of Engineering, Hyderabad, IndiaAbstract:- This paper presents the results of an experimental research on the workability andmechanical properties of self-compacting concrete. The work focused on concrete mixes havingWater/Cement ratios of 0.23, 0.24, 0.25, 0.26 and 0.27, with a Packing Factor of 1.12. The Concretemixes contains different proportions of GGBS, Super plasticizers, water binder ratios and constantproportions of Cement, Micro Silica, VMA, Coarse aggregate and Fine aggregate for different WaterCement ratios. The percentage of Micro Silica added is 7% for all mixes. The mix proportions areobtained on the basis of NAN-SU mix design. All the mixes contain Cement of 574 kg/m3but withdifferent total binder content. The workability tests performed in this research were as per EFNARC.Based upon the experimental results, for water cement ratio 0.25 fresh and hardened state properties ofhigh strength self-compacting concrete are moderate.Keywords:- Self-Compacting Concrete, Workability, GGBS, Micro silica, Super plasticizer andVMA.I. INTRODUCTIONSelf-compacting concrete having advanced viscosity and workability properties can easily fill themoulds without the necessity of using vibrators. High volume of mineral powder is a necessity for a proper self-compacting concrete design. For this purpose, mineral admixtures such as limestone powder, Fly Ash, microsilica, rice husk ash and blast furnace slag can be used. In this study, the effect of water cement ratio on freshand hardened properties of self -compacting concrete has been investigated.It is worth noting that extensive investigations on the workability of self-compacting concrete havebeen made recently. Kayat et al. reported that the L-box, U-box, and J-ring tests can be used to evaluate thepassing ability of self-compacting concrete and to a certain extent, the deformability and resistance tosegregation. When combined with the slump flow test, the L-box test is very suitable for the quality control ofon-site self-compacting concrete.It is apparent that workability depends on a number of interacting factors such as water content,aggregate type and grading, fine aggregate to coarse aggregate ratio, packing factor, kind and dosage of superplasticizers, and the fineness of cement. The main factors on self-compacting concrete are the water and superplasticizer contents of the mix since by simply adding them the inter particle lubrication is increased.In this research mix design used is based on NAN-SU method. His design is based on packing factor(PF) of aggregate. In this research PF and FA/CA used are 1.12 and 52/48 for different W/C ratios. Proportionsof GGBS, Super plasticizers and water binder ratios are different and proportions of Cement, Micro Silica,VMA, Coarse aggregate and Fine aggregate are constant for different Water Cement ratios. The percentages ofMicro Silica and VMA added are 7% and 0.3% for all mixes.II. MATERIALS AND MIX PROPORTIONSThis part of the paper presents the specifications of the mixes used for obtaining the workability,compressive strength, split tensile strength and flexural strength of self-compacting concrete. Ordinary PortlandCement (OPC 53 grade), GGBS and Micro silica were used as cementitious materials. Natural river sand andcrushed gravel with a nominal maximum size of 10 mm were used as the aggregates. Chemical admixtures usedwere GLENIUM B233 (a new generation based on modified poly carboxylic ether) as super plasticizer andGlenium Stream-2 as VMA.
Effect of W/C Ratio on Workability and Mechanical Properties of High…7Table 1: Mix proportions of concrete containing different water to cement ratios.MixComponentsConcrete MixesM1W/C=0.23M2W/C=0.24M3W/C=0.25M4W/C=0.26M5W/C=0.27Qty.(kg/m3)Qty.(kg/m3)Qty.(kg/m3)Qty.(kg/m3)Qty.(kg/m3)Cement 574 574 574 574 574GGBS 54.57 45.65 36.73 27.82 18.9Miro Silica 40.18 40.18 40.18 40.18 40.18F.Aggregate 844.48 844.48 844.48 844.48 844.48C.Aggregate 805.32 805.32 805.32 805.32 805.32Water/Binder 140.83 143.65 146.83 150.01 153.18SuperPlasticisers11.31 11.15 10.99 10.83 10.67VMA 1.722 1.722 1.722 1.722 1.722III. WORKABILITY AND COMPRESSIVE STRENGTHThe strict definition of workability is the amount of useful internal work necessary to produce fullcompaction. The useful internal work is a physical property of concrete and is the work or energy required toovercome the internal friction between the individual particles of the mixture. Because of the very highworkability of self-compacting concrete, it needs no external vibration and can spread into place, fill theframework and encapsulate reinforcement without any bleeding or segregation. In other words, to ensure thatreinforcement can be encapsulated and that the framework can be filled completely, a favourable workability isessential for self-compacting concrete. Moreover, aggregate particles in self compacting concrete are required tohave uniform distribution in the specimen and the minimum segregation risk should be maintained during theprocess of transportation and placement.Because the strength of concrete is adversely and significantly affected by the presence of voids in thecompacted mass, it is vital to achieve a maximum possible density. This requires a sufficient workability orvirtually full compaction. It is obvious that the presence of voids in concrete reduces the density and greatlyreduces the strength, which means the presence of 5 percent of voids can lower the strength by as much as 30percent. This research compares the compressive strength, split tensile strength and flexural strength of selfcompacting concrete mixtures for different water cement ratios.IV. RESULTS AND DISCUSSIONIn this part of the paper, the experimental results of self-compacting concrete mixes related tocompressive strength, split tensile strength, flexural strength and workability are discussed for different watercement ratios. The workability tests performed in this research were as per EFNARC methods. They are Slumpflow, L-box, U-box and V-funnel.A. Experimental ResultsThe results of workability tests on self-compacting concrete are shown in Table 2. It can be observedthat as the W/C ratio increases the workability increases. The results of compressive strength, split tensilestrength and flexural strength are shown in Table 3.It can be observed that the strengths are decreasing withincrease in W/C ratio.B. Fresh and hardened state properties of Self-compacting concreteSlump Flow (SF) increases as the w/c ratio increases. When w/c increases from 0.23 to 0.27(17.4%) ,slump flow increases from 650mm to 675mm(3.8%). (Figure 1)T500, V-funnel, T5 and U-box values are decreasing as the w/c ratio increases. When w/c ratioincreases from 0.23 to 0.27(17.4%), T500 time decreases from 4.74 sec to 3.97 sec (16.24%),V-funnel timedecreases from 11.4sec to 9.77sec (14.3%), T5 time decreases from 14.60sec to 11.87sec(18.69%) and U-boxvalue decreases from 13mm to 5mm (61.53%). It is observed that workability increases as the w/c ratioincreases. (Figures 2, 3, 4 and 6)L-box value increases as the w/c ratio increase. When w/c ratio increases from 0.23 to 0.27(17.4%), L-box ratio increases from 0.94 to 0.97(3.19%).It is observed that flow ability increases as the w/c ratio increases.(Figure 5)
Effect of W/C Ratio on Workability and Mechanical Properties of High…8Compressive strength decreases as the w/c ratio increases. When w/c ratio increases from 0.23 to0.27(17.4%), 7days Compressive strength decreases from 60.44MPa to 51.88MPa (14.16%). Whereas 28daysCompressive strength decreases from 83.42MPa to 81.43MPa (2.38%). (Figure 7)Split tensile strength decreases as the w/c ratio increases. When w/c ratio increases from 0.23 to0.27(17.4%), 7days Split tensile strength decreases from 3.66MPa to 3.27MPa (10.65%). Whereas 28days Splittensile strength decreases from4.367MPa to 3.97MPa (9.09%). (Figure 8)Flexural strength decreases as the w/c ratio increases. When w/c ratio increases from 0.23 to0.27(17.4%), 7days Flexural strength decreases from 5.72MPa to 5.15MPa (9.96%).Where as 28days Flexuralstrength decreases from 6.58MPa to 5.65MPa (14.13%). (Figure 9)It is observed that Compressive strength and Split tensile strength decreases at higher rate for 7daysstrength when compared to 28days strength, where as the Flexural strength decreases at higher rate for 28daysstrength when compared to 7days strength.The relation between the strengths and water cement ratios are as given below.fck = -47.6 ( ) + 94.466ft = -9.64 ( ) + 6.5814fcr = -25.2 ( ) + 12.418Wherefck = 28 days compressive strength in MPa.ft = 28 days split tensile strength in MPa.fcr = 28 days flexural strength in MPa.= water cement ratio.The relation between the flow values and water cement ratios are as given below.S.F in mm = 630 ( ) + 504.5T500 in sec = -16.3 ( ) + 8.315V-funnel in sec = -42.6 ( ) + 21.204T5 in sec = -66.6 ( ) + 30.054L-box ratio = 0.75 ( ) + 0.7655U-box ratio = -210 ( ) + 61.1The relation between Compressive strength and Flexural strength is as given below. (Figure 10)fcr = 0.5017 ( fck ) – 35.309The relation between Compressive strength and Split tensile strength is as given below. (Figure 11)ft = 0.1972 ( fck ) – 12.113Table 2: Workability of the concrete mixesWorkabilityTestsConcrete MixesM1 W/C=0.23 M2 W/C=0.24 M3 W/C=0.25 M4 W/C=0.26 M5 W/C=0.27Slump flow(mm)650x650 655x655 662x662 668x668 675x675T 500(sec) 4.74 4.21 4.16 4.12 3.97
Effect of W/C Ratio on Workability and Mechanical Properties of High…9V-funnel(sec)11.4 11.1 10.4 10.1 9.77V-funnelT5 min(sec)14.60 14.11 13.53 12.91 11.87L-box(h2/h1)0.94 0.945 0.95 0.96 0.97U-box (mm) 13 11 8 6 5Table 3: Development of compressive strength, split tensile strength and flexural strength with ageConcrete Mix Compressive strength(N/mm2)Split tensile strength(N/mm2)Flexural strength(N/mm2)7days 28days 7days 28days 7days 28daysM1W/C=0.2360.44 83.42 3.66 4.367 5.72 6.58M2W/C=0.2459.03 83.07 3.56 4.27 5.64 6.42M3W/C=0.2554.21 82.62 3.39 4.15 5.32 6.18M4W/C=0.2652.13 82.29 3.33 4.1 5.25 5.76M5W/C=0.2751.88 81.43 3.27 3.97 5.15 5.65Figure 1: w/c ratio Vs slump flowFigure 2: w/c Ratio Vs T500
Effect of W/C Ratio on Workability and Mechanical Properties of High…10Figure 3: w/c Ratio Vs V-funnel0.940.9450.950.960.970.930.940.950.960.970.980.22 0.23 0.24 0.25 0.26 0.27 0.28L-BoxRatioW/C RatioL-Box ratioL-Box ratioFigure 4: w/c Ratio Vs L-Box Ratio131186 50510150.22 0.23 0.24 0.25 0.26 0.27 0.28U-BoxRatioW/C RatioU-BoxU-BoxFigure 5: w/c Ratio Vs U-Box
Effect of W/C Ratio on Workability and Mechanical Properties of High…1183.42 83.07 82.62 82.29 81.4360.44 59.03 54.21 52.13 51.880204060801000.22 0.23 0.24 0.25 0.26 0.27 0.28CompressiveStrengthinMPaW/C RatioCompressive StrengthCompressivestrength(28days)Compressivestrength(7days)Figure 6: w/c Ratio Vs Compressive strength4.367 4.27 4.15 4.1 3.973.66 3.56 3.39 3.33 3.270123450.22 0.23 0.24 0.25 0.26 0.27 0.28SplitTensileStrengthinMPaW/C RatioSplit Tensile StrengthSplit tensilestrength(28days)Split tensile strength(7days)Figure 7: w/c Ratio Vs Split tensile strengthFigure 8: w/c Ratio Vs Flexural strength
Effect of W/C Ratio on Workability and Mechanical Properties of High…124.3674.2220.127.116.113.918.104.22.168.481 81.5 82 82.5 83 83.5 84SplitTensileStrengthCompressive StrengthSplit tensile strengthSplit tensile strengthFigure 11: Compressive Strength Vs Split Tensile strengthIV. CONCLUSIONSFrom the results presented in this paper using self compacting concrete with different w/c ratios forconstant packing factor, the main conclusions are1. Required minimum slump is achieved for a w/c ratio of 0.23 with optimum strength for M70 grade highstrength self compacting concrete.2. Required minimum strengths are achieved for a w/c ratio 0.27 with optimum slump for M70 grade highstrength self compacting concrete.3. For water cement ratio 0.25 fresh and hardened state properties of high strength self-compacting concreteare moderate.4. These values are obtained for a Packing Factor of 1.12 with addition of 7% micro silica.REFERENCES. Anne-Meike Poppe an Geert De Schutter. “Cement hydration in the presence of high filler contents”.Cement and Concrete research 2005, Vol.35, pp 2290-2299.. Buia, V.K., Montgomeryb, D., Hinczak, I. and Turner, K. “Rapid testing method for segregationresistance of self-compacting concrete,” Cement and Concrete Research, Vol.32, 2002, pp 1489-1496.. Celik Ozyildirim, Stephen Lane D, “Measurement of properties of fresh self compacting concrete “Final report, Europian Union Growth Contact No. G6RD-CT-2001-00580,Sepetember 2005 pp 1489 -1496.. Collepardi.M., “Self –compacting concrete: What is new? “ Poceeding of the seventh CANMET/ACIConference on Superplasticisers and other chemical dmixtures in concrete, Berlin(Germany), 2003, pp.1-16.. Domone, P.L. “A review of the hardened mechanical properties of self-compacting concrete,”Cementand Concrete Composites, 29, 2007, 1-12.. European Project Group, Specification and guidelines for self-compacting concrete, United Kingdom,. EFNARC, 2002.. Felekoglu, B. “Investigation on mechanical and physical properties of SCC,” M.Sc. Thesis in CivilEngineering, Dokus Eylul University, Izmir, 2003.  Felekoglu, B., Turkel, S. and Baradan, B.“Effect of water/cement ratio on the fresh and hardened properties of self-compacting concrete,”Building and Environment, 42, 2007, 1795-1802.. Felekoglu, B. and Sarikahya, H. “Effect of chemical structure of polycarboxylate-basedsuperplasticizers on workability retention of self-compacting concrete,” Construction and BuildingMaterials, 22, 2008, 1792-1980.. Gibbs JC, Zhu W. “Strength of hardened self compacting concrete”. In the 1stInternational RILEMSymposium on Self-compacting concrete, 1999. Skarendahl.A. Petersson.O.,editors, RILEMPublications S.A.R.L., PP 199-209.. Gomes.P.C.C, Ravindra Gettu et al., “Experimental optimisation of High Strength Self CompactingConcrete”, proceedings of the second international conference on Self Compacting Concrete, Tokyo,October 2001.. Hemant Sood, Khitoliya R.K. and Pathak .S., “ Incorporating European Standards for testing selfcompacting concrete in Indian conditions”. International Journal of Recent Trends in Engineering May2009, Vol.1, No.6, pp 41-45.
Effect of W/C Ratio on Workability and Mechanical Properties of High…13. Khatri, R.P. and Sirivivatnanon, V. “Effect of different supplementary cementitious materials onmechanical properties of high performance concrete,” Cement and Concrete Research, 25, 1, 1995,209-220.. Lachemia M., Hossiana K.M.A, Lambrosa V., Nkinamubanzib and Bouzoubaa N. “Performance ofnew viscosity modifying admixtures in enhancing the rheological properties of cement paste”. Cementand concrete research, 2004, Vol.34, pp 185-193.. Nan Su, Kung –Chung Hsub and His-Wen Chai. “ A simple mix design method for self compactingconcrete”. Cement and Concrete Research, 2001, Vol.31, pp 1799-1807.. Su, N. and Miao,B. “A new method for mix design of medium strength flowing concrete with lowcement content,” Cement and Concrete Composites, 25, 2003, 215-222.. Okamura, H. and Ouchi, M. “Self-compacting concrete: development, present use and future,”Proceedings of the First International RILEM Symposioum , 1999, 3-14.. Okamura, H. and Ouchi, M. “Self-compacting concrete”. Journal of advanced concrete technology,2003, Vol.1, No.1, pp 5-15. Ravindra Krishna M. “ Strength and durability behaviour of super plasticized high strength concreteusing combination of mineral admixtures”, PhD thesis of JNTUH, 2005.. Subramanian, S. and Chattopadhyay D. “Experiments for mix proportioning of Self – compactingconcrete”, The Indian Concrete Journal, 2002, pp.13-20.. S. Venkateswara Rao, M. V. Seshagiri Rao and P. Ratihish Kumar. “Effect of size of aggregate andfines on standard and high strength self-compacting concrete”, Applied science research, 6(5): 433-442, 2010.